antibacterial efficacy of ultrahigh molecular weight ... (varioklav¢®, h + p labortechnik,...
Post on 26-Jan-2021
Embed Size (px)
Harrasser et al. AMB Expr (2015) 5:64 DOI 10.1186/s13568-015-0148-x
Antibacterial efficacy of ultrahigh molecular weight polyethylene with silver containing diamond-like surface layers Norbert Harrasser1, Sebastian Jüssen1, Ingo J. Banke1, Ralf Kmeth2, Ruediger von Eisenhart‑Rothe1, Bernd Stritzker2, Hans Gollwitzer1,3 and Rainer Burgkart1*
Abstract Antibacterial coating of medical devices is a promising approach to reduce the risk of infection but has not yet been achieved on wear surfaces, e.g. polyethylene (PE). We quantitatively determined the antimicrobial potency of differ‑ ent PE surfaces, which had been conversed to diamond‑like carbon (DLC‑PE) and doped with silver ions (Ag‑DLC‑ PE). Bacterial adhesion and planktonic growth of various strains of S. epidermidis on Ag‑DLC‑PE were compared to untreated PE by quantification of colony forming units on the adherent surface and in the growth medium as well as semiquantitatively by determining the grade of biofilm formation by scanning electron microscopy. (1) A significant (p < 0.05) antimicrobial effect could be found for Ag‑DLC‑PE. (2) The antimicrobial effect was positively correlated with the applied fluences of Ag (fivefold reduced bacterial surface growth and fourfold reduced bacterial concentration in the surrounding medium with fluences of 1 × 1017 vs. 1 × 1016 cm−2 under implantation energy of 10 keV). (3) A low depth of Ag penetration using low ion energies (10 or 20 vs. 100 keV) led to evident antimicrobial effects (fourfold reduced bacterial surface growth and twofold reduced bacterial concentration in the surrounding medium with 10 or 20 keV and 1 × 1017 cm−2 vs. no reduction of growth with 100 keV and 1 × 1017 cm−2). (4) Biofilm formation was decreased by Ag‑DLC‑PE surfaces. The results obtained in this study suggest that PE‑surfaces can be equipped with antibacterial effects and may provide a promising platform to finally add antibacterial coatings on wear surfaces of joint prostheses.
Keywords: Implant‑associated infections, Diamond‑like carbon, Silver, Staphylococcus epidermidis, Antibacterial coating
© 2015 Harrasser et al. This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
Introduction The great success of surgically-implanted biomateri- als may be compromised in every case by the challeng- ing complication of bacterial periimplant infection (Liu et al. 2012; Zimmerli and Ochsner 2003). Approximately 2.6 million orthopedic biomaterials are implanted annu- ally in the USA, hence the incidence of implant-asso- ciated infections is also increasing (Kurtz et al. 2008). Most important in the pathogenesis of infection is the
colonization of the device surface and the consecu- tive formation of a biofilm (Zimmerli and Moser 2012; Gosheger et al. 2004), in which Staphylococcus aureus and koagulase-negative Staphylococci are most fre- quently implicated as the etiologic agents (Zimmerli and Ochsner 2003; Hunter and Dandy 1977). Prevention of these infections has an important impact not only on patient’s morbidity but also on the cost effectiveness of hospital care (Gosheger et al. 2004). Systemic antibiotic prophylaxis and various local antibiotic delivery tech- niques have been proven to reduce the rate of infec- tion (Gollwitzer et al. 2003; Schmidmaier et al. 2006). Hereby locally applied antibiotics are advantageous in delivering high drug concentrations to the required site without producing systemic toxicity (Zhang et al. 2014).
*Correspondence: email@example.com 1 Clinic of Orthopedics and Sports Orthopedics, Klinikum rechts der Isar, Technical University of Munich, Ismaninger Str. 22, 81675 Munich, Germany Full list of author information is available at the end of the article
Page 2 of 9Harrasser et al. AMB Expr (2015) 5:64
Because pathogens involved in implant associated infec- tions are diverse and bacteria in biofilms are protected from antibiotics (Ceri et al. 1999), the restricted activ- ity of these substances limits their clinical effectiveness, especially in infections involving antibiotic-resistant bacterial strains (e.g. MRSA) (Liu et al. 2012). There- fore, alternatives to local antibiotic delivery systems are highly favored. In this context employment of implant materials or coatings that control infection and biofilm formation would be particularly advantageous (Schmid- maier et al. 2006). This led to the development of anti- adhesive and non-antibiotic antibacterial surfaces. The first mentioned coatings (e.g. polyethylene glycol, poly- ethylene oxide brushes) reduce bacterial adhesion by altering the physicochemical properties of the substrate. Thus, formation of protein surface layers (conditioning films) on the implant and bacteria–substrate interac- tions are hindered (Hetrick and Schoenfisch 2006). This mode of action is referred to as ‘‘passive’’. However the effectiveness of these coatings for reducing bacterial adhesion is very limited and varies greatly depending on bacterial species. Additionally, osseointegration is poor. In sum, the importance of these antiadhesive coatings in orthopedic surgery is limited. In contrast non-antibi- otic “active” antibacterial coatings release antibacterial agents, e.g. silver ions (Ag+), copper ions (Cu++), nitric oxide, chlorhexidine/chloroxylenol or chitosan (Kumar and Munstedt 2005; Hardes et al. 2007; Gosheger et al. 2004; Shirai et al. 2009). Compared to antibiotics these agents act more broadly against a wide range of bacteria. In addition, at least proven for the use of Ag+, microbes without intrinsic resistance cannot gain resistance (Kumar and Munstedt 2005; Lee et al. 2005).
So far, these antibacterial coatings have not been applied on soft wear surfaces, e.g. polyethylene (PE). In total knee replacement roughly half of the surface is exposed to synovial fluid and in main parts tribologi- cally active. Therefore in septic revision surgery major portions of the susceptible prosthesis are not protected against bacterial reinfection. Antibacterial-agent- enriched diamond-like carbon (DLC) surfaces may solve this dilemma. By release of Ag+ these surfaces could act as local antibacterial agents (Cloutier et al. 2014; Katsiko- gianni et al. 2006). At the same time appropriate DLC surfaces can exhibit excellent tribological features as already shown for hip or knee arthroplasty (Saikko et al. 2001; Dearnaley 1993; Oliveira et al. 2014).
In this study the antimicrobial effects of silver (Ag) incorporated DLC surfaces on PE (Ag-DLC-PE) are investigated. PE was chosen due to its outstanding importance in orthopedic surgery as a wear surface. This study provides valuable information for determining the suitability of Ag-DLC-PE for septic revision surgery.
Materials and methods Study substrates and surface conversion Study objects were cylindrical substrates (diameter: 10 mm, height: 2 mm; Goodfellow GmbH, Nauheim, Germany) of PE (ultrahigh molecular weight PE, UHM- WPE). DLC-processing of the plates was performed at the Department of Experimental Physics IV, University of Augsburg (Germany). The samples were treated accord- ing to a modified technique of ion irradiation of poly- mers, in which DLC-processing was achieved by direct ion bombardment of Ag+ or nitrogen (Bertóti et al. 2007). In contrast to common DLC techniques, the PE surface is not coated with DLC but rather modified by silver ion implantation. Due to the kinetic energy of the implanted Ag+, the polymer surface is modified from crystalline PE to amorphous DLC, while the metal ions agglomerate to Ag nano-particles directly under the surface. In this way, the implantation of silver ions leads to a wear-resistant, silver-containing modified PE surface reducing the risk of detachment compared to surface coatings (Fig. 1) (Schwarz and Stritzker 2010).
These surface conversed DLC-PE samples were inves- tigated in three groups with modified parameters of Ag+-implantation: firstly, to determine the influence of different ion energies (first group) and secondly, to deter- mine the influence of different fluences (second group). In order to elucidate which of these factors (ion energy vs. fluence) has a major impact on microbes a third test- ing group was conducted. All sample features and testing groups are given in Table 1.
In the first group three Ag-doped samples with con- stant fluences (1 × 1017 cm−2) and different ion energies (60, 80, 100 keV) were assembled. DLC processing was carried out via direct ion implantation of Ag+. Based on the findings of the first group the second group was
Fig. 1 Transmission electron microscopy (TEM) image of silver nanoparticles of AG‑DLC‑PE; notice nanoparticles do not coat the PE surface but are embedded in the PE
Page 3 of 9Harrasser et al. AMB Expr (2015) 5:64
performed with three different fluences of Ag+ (1 × 1016, 5 × 1016 and 1 × 1017 cm−2) and constant low implan- tation energy (10 keV). In the third group samples were subjected to ion bombardment of Ag+ with different flu- ences and low ion energies (20 keV: 5 × 1016 and 1 × 1017 cm−2; 10 keV